Reactive & Functional Polymers 68 (2008) 1307–1313 Contents lists available at ScienceDirect Reactive & Functional Polymers journal homepage: www.elsevier.com/locate/react Preparation of epoxy-modiﬁed polyethylene by graft extrusion and its applications to polyphenylene sulﬁde alloys as a compatibilizer Chen-Ming Chen a, Tsung-Eong Hsieh a,*, Mark O. Liu b a b Department of Materials Science and Engineering, National Chiao Tung University, Hsinchu 300, Taiwan, ROC Material and Chemical Research Laboratories, Industrial Technology Research Institute, Hsinchu 300, Taiwan, ROC a r t i c l e i n f o Article history: Received 20 December 2007 Received in revised form 17 May 2008 Accepted 14 June 2008 Available online 21 June 2008 Keywords: Epoxy-modiﬁed polyethylene Graft extrusion Compatibilizer a b s t r a c t Epoxy-modiﬁed polyethylene (PE-g-GMA) was successfully synthesized from glycidyl methacrylate (GMA) and low-density polyethylene (LDPE) via the grafting reaction of extrusion. The mechanism of grafting reaction and the rapid determination for the percentage of grafting are also reported. Experimental results demonstrated that the PE-g-GMA is a good compatibilizer in polyphenylene sulﬁde/poly(ethylene terephthalate) (PPS/PET) as well as PPS/nylon 6,6/glass ﬁber alloys and the addition of PE-g-GMA into PPS alloys may effectively improve the mechanical properties of composites. Ó 2008 Elsevier Ltd. All rights reserved. 1. Introduction Polyethylene (PE) is a versatile polymer [1,2] and its chemical reactivity can be modiﬁed by means of grafting various functionalized monomers onto its backbone without substantial loss of its physical properties. The grafting process may be carried out in solution or molten PE with copolymerization of methyl methacrylate, maleic anhydride, styrene, acrylic acid, and trimethoxysilane [1–4]. The chemically modiﬁed PE has extensive applications especially as a compatibilizer for polymer alloys . Although the grafting reaction of PE can be executed by conventional reactors, the process takes several hours for completion and is batch-producing [6–8]. However, the extrusion procedure is fast and continuous, being more suitable for industrial mass production. In this work, glycidyl methacrylate (GMA) was grafted to low-density polyethylene (LDPE) with initiators by reactive extrusion procedure in a twin screw extruder. The grafted product (PE-g-GMA) was subsequently analyzed by means of FTIR spectra as well as the element analysis. The linear * Corresponding author. Tel.: +886 3 5712121 55306; fax: +886 3 5724727. E-mail address: [email protected] (T.-E. Hsieh). 1381-5148/$ - see front matter Ó 2008 Elsevier Ltd. All rights reserved. doi:10.1016/j.reactfunctpolym.2008.06.008 calibration curve was drawn for a rapid estimation of the percentage of grafting. Moreover, the dependence of the percentage of grafting on processing parameters was also investigated in detail. Finally, the PE-g-GMA was added in polyphenylene sulﬁde/poly(ethylene terephthalate) (PPS/ PET) and the PPS/nylon 6,6/glass ﬁber alloys to serves as a compatibilizer and a successful enhancement on their mechanical properties was obtained. 2. Experimental 2.1. Materials The LDPE pellet (NA 20766), whose density and melt index are 0.923 g/cm3 and 8 g/10 min, respectively, was supplied by USI Far East Co. of Taiwan. The GMA, PET, PPS (P-4), nylon 6,6, and PE-g-Acrylic acid (PB1009), whose chemical structures were shown in Fig. 1, were obtained from Japanese Oil and Fat Co., Shinkong Synthetic Fibers Co., Du Pont Co., Phillips Petroleum Co., and BP Performance Polymer Inc., respectively. The initiator (2,5dimethyl-2,5-bis(t-butyl-peroxy)hexane (TX 101) as shown in Fig. 1) with a half-life of approximately 6 min at 160 °C was purchased from the Akzo Chemie Co. 1308 C.-M. Chen et al. / Reactive & Functional Polymers 68 (2008) 1307–1313 O CH2 O C H2 C O C2 H 4 O O O O C C n C PET CH3 GMA O H N S H N (CH2)6 C O ( CH2)4 C n n PPS nylon 6,6 CH2 C H2 CH2 CH m n CH2 O CH C O H x PE-g-Acrylic acid H3C H3C CH3 OO CH3 CH3 OO CH2 CH3 CH3 CH3 CH3 CH3 TX 101 Fig. 1. The chemical structures of GMA, PET, PPS, nylon 6,6, PE-g-Acrylic acid, and TX 101. 2.2. Grafting process of GMA and LDPE 2.3. Preparation and characterizations of PPS alloys The grafting reaction was manifested in Scheme 1 and carried out by using a twin screw extruder (W&P, ZSK 25). The LDPE pellets were fed at 40 g/min into the hopper and the GMA/TX 101 solution was injected into the twin screw extruder from the injection nozzle via a liquid chromatography pump. The extrudate was pelletized and then dried prior to analysis. The crude polymer was dissolved in hot toluene, precipitated the product with methanol, and then dried in reduced pressure at 50 °C for 24 h. The element analyzer (Heraeus CHN-0-Rapid F002) was used to analyze the contents of oxygen of the dried polymer. Thin ﬁlm samples for Fourier-transform infrared (FTIR) analysis were prepared by pressing the precipitated resin between two mylar sheets at 120 °C and 5000 kg/cm2 for 1 min. FTIR measurements were performed by using a Bio-Rad Digitlab Division UMA 300/FTS-40 spectrometer. The thermalgravimetric analysis (TGA) was carried out by using a Perkin–Elmer TGA7 and in temperatures ranging from room temperature to 470 °C at a heating rate of 10 °C/min in nitrogen ambient. PPS powder, PET or nylon 6,6 pellets/glass ﬁber, and the compatibilizer (PE-g-GMA) were mixed in the twin screw extruder at 280 °C at a screw speed of 300 rpm. The extrudate was then cooled and pelletized. Impact test specimens were prepared by an injection molding machine (Toshiba IS55). Izod impact test was conducted on unnotched specimens at 25 °C according to ASTM D256 test standard. Morphologies of fractured surfaces of PPS/PET alloys were examined by scanning electron microscopy (SEM, Cambridge model S360). 3. Results and discussion 3.1. The mechanism of grafting reactions Fig. 2 depicts the possible reactions taking place during grafting procedure . First, the primary R radical produced by thermal decomposition of TX 101 extracts a hydrogen atom from PE chains (reaction (1)). The radicals generated by peroxide decomposition then attack PE, 1309 C.-M. Chen et al. / Reactive & Functional Polymers 68 (2008) 1307–1313 O CH2 O H2C C O C + CH3 GMA CH2 TX 101 CH2 n C H2 extruder CH2 CH2 CH m n LDPE CH2 PE-g-GMA O C C CH3 x O CH2 O Scheme 1. Fig. 2. Overview of the free radical reactions. preferentially at branch chain, to produce PE, which either undergo crosslinking or disproportionation (reaction (2)). Simultaneously, the homopolymerization of GMA occurs, yielding (GMA)n which undergoes chain transfer to form PE (reactions (3) and (4)). These reactive sites of PE backbone either react with GMA or capture (GMA)n, and ﬁnally result in grafting reactions (reactions (5) and (6)). Among these possible reactions, reaction (5) is the key reaction for the grafting process of LDPE and GMA. 3.2. Estimation of the percentage of grafting The FTIR spectra of pure LDPE and PE-g-GMA are presented in Fig. 3a and b, respectively. As shown in Fig. 3b, the absorption bands at 846, 908, and 995 cm 1 are the characteristic vibrations of epoxy groups , indicating the occurrence of grafting reaction (Scheme 1). As to the percentage of grafting (%grafting), it can be directly calculated by the ratio of the absorbance of the carbonyl group for PE-g-GMA to that of the methylene group for pure LDPE. However, this method is tedious. In order to simplify the determination of %grafting, we draw the calibration curve  in terms of the experimental results of extrudates a, b, c, and d (Table 1) as shown in Fig. 4, whose abscissa is the ratio of carbonyl stretch (mCO, 1731 cm 1) to the methyl stretch (dCH3, 1376 cm 1) for PE-g-GMA (i.e., mCO/dCH3) and ordinate is the content of oxygen for PE-g-GMA (%oxygen), respectively. The mCO/ dCH3 and %oxygen are measured by FTIR and element analysis, respectively. Since the linear calibration curve has been successfully established, the %grafting can be rapidly estimated from the %oxygen as shown in Fig. 4, whose acquirement is much easier than mCO/dCH3, through ﬁtting of the linear calibration curve. For example, in case of extrudates e, we obtain %oxygen (0.16) from the FTIR result and then the %grafting can be determined to be 0.48 by matching the calibration curve (Fig. 4). 1310 C.-M. Chen et al. / Reactive & Functional Polymers 68 (2008) 1307–1313 Absorbance (%) a 0.30 0.25 0.20 0.15 0.10 0.05 0.00 4000 3500 3000 2500 2000 1800 1600 1400 1200 1000 800 600 400 Wavenumbers (cm−1) Absorbance (%) b 0.30 0.25 0.20 0.15 0.10 0.05 0.00 4000 3500 3000 2500 2000 1800 1600 1400 1200 1000 800 600 400 −1 Wavenumbers (cm ) Fig. 3. The FTIR spectra of (a) pure LDPE and (b) PE-g-GMA. Table 1 Summary of the experimental results of grafting reactions Extrudate Composition of LDPE/GMA/TX101 (wt./wt./wt.) Screw speed (rpm) Processing temp. (°C) mCO/dCH3 %Oxygen %Grafting a b c d e f g h i j k l 100/40/0.2 100/20/0.8 100/30/1 100/5/2 100/10/0.27 100/10/0.53 100/10/0.80 100/10/0.53 100/10/0.53 100/15/0.27 100/15/0.27 100/15/0.27 100 200 300 100 200 200 200 300 100 200 200 200 120 200 220 275 220 220 220 220 220 220 145 255 2.49 2.44 2.98 0.96 – – – – – – – – 1.42 1.45 1.75 0.60 0.16 0.21 0.28 0.11 0.26 0.20 0.05 0.58 4.20 4.29 5.18 1.78 0.48 0.62 0.82 0.33 0.77 0.59 0.14 1.72 3.3. Dependence of processing parameters on grafting reaction of extrusion As shown in Table 1, the %grafting is strongly dependent on the processing parameters such as concentration of initiator, screw speed, concentration of GMA, and processing temperature. In case of the extrudates e, f, and g, %grafting increases with the rising of concentration of initiator (TX 101), revealing higher concentration of TX 101 promotes the initiation of grafting reaction (reaction (1) of Fig. 2) and raises the %grafting. Furthermore, a comparison of the experimental results of extrudates f, h, and i indicates the %grafting decreases with the increase of screw speed, revealing the faster screw speed shortens the residence time of reactants in the extruder and thus reduces the %grafting. In case of extrudates e and j, %grafting rises with the raising of concentration of reactant (GMA). In addition, it was also found that the processing temperature highly inﬂuences the %grafting. As shown in the experimental results of extrudates j, k, and l, the %grafting heightens with the increase of the processing temperature; manifesting higher temperature causes higher speed and yield of grafting reaction. Therefore, we can ingeniously manipulate the %grafting by the modulation of processing parameters. In the near future, we will keep on analyzing the inﬂuence of the grafting procedure on grafting efﬁciency by statistical methods to acquire more detailed results. 3.4. PE-g-GMA as the compatibilizer of PPS Alloys 3.4.1. Thermal properties of PE-g-GMA PPS alloys have been produced before with appropriate commercially available compatibilizers (e.g. PE-g-Acrylic acid, PE-g-maleic anhydride, etc.) [12–14]. However, these 1311 C.-M. Chen et al. / Reactive & Functional Polymers 68 (2008) 1307–1313 2.0 5.90 1.8 1.6 % OXYGEN 1.2 3.54 1.0 0.8 2.36 % GRAFTING 4.72 1.4 0.6 0.4 1.18 0.2 0.0 0.00 0.0 0.6 1.2 1.8 2.4 3.0 3.6 υCO/δCH3 Fig. 4. The calibration curve for PE-g-GMA. tions and the mechanical properties of the PPS/PET alloys are tabulated in Table 2. The experimental results illustrate that the unnotched impact strength of PPS/PET alloys with PE-g-GMA (alloy n) is higher than that without PE-g-GMA (alloy m), indicating the introduction of PE-g-GMA is capable of promoting the mechanical properties. Furthermore, the improvement of compatibility for PPS/PET alloys could be deduced from the results of SEM observation. As shown compatibilizers exhibit poor thermal stability, limiting the application of PPS alloys. Fig. 5 illustrates the TGA curve of PE-g-GMA. In case of PE-g-GMA, no degradation occurred until 300 °C in nitrogen ambient and its decomposition temperature could reach 372 °C. In comparison with the commercially available compatibilizer (PE-g-Acrylic acid), PE-g-GMA apparently exhibits a superior thermal stability since the epoxy group in PE-g-GMA can be more effective in resisting the heat than the carboxyl acid group of PEg-acrylic acid. This result reveals that PE-g-GMA is a better compatibilizer for alloys of high performance engineering plastics, e.g., PPS/PET or PPS/nylon 66, etc., than PE-g-Acrylic acid. Table 2 Summary of the experimental results of PPS/PET alloys 3.4.2. PE-g-GMA as a compatibilizer of PPS/PET and PPS/ Nylon 6,6/Glass ﬁber alloys The PPS, PET and PE-g-GMA were blended in the twin screw extruder and the specimens for subsequent tests were prepared by injection molding. The blend composi- Alloy Composition of PPS/PET/PE-g-GMA (wt./wt./wt.) Unnotched impact strength (kg/cm)a m n 100/50/0 100/50/12.5 6.81 10.0 a Measured at 25 °C after aging at 240 °C for 231 h (the standard deviations = ±2%). 110 Weight (%) 90 70 50 30 10 -10 100 150 200 250 300 350 400 450 500 Fig. 5. The TGA cueves of PE-g-GMA and PE-g-Acrylic acid in nitrogen ambient. 1312 C.-M. Chen et al. / Reactive & Functional Polymers 68 (2008) 1307–1313 Fig. 6. SEM micrographs of PPS/PET alloys: (a) without PE-g-GMA (b) with the PE-g-GMA. in Fig. 6a, alloy m exhibits the morphology with an incompatible phenomenon, while alloy n (Fig. 6b) exhibits the morphology with ﬁne and uniform dispersion, manifesting the enhancement of the compatibility between PPS and PET by PE-g-GMA since the epoxy group of PE-g-GMA may attract with the carboxyl as well as oxygen groups of PET and the sulﬁde group of PPS via strong van der Waal forces. In order to further raise the mechanical properties of PPS, we also introduced nylon 6,6 and glass ﬁber into the PPS to form PPS/nylon 6,6/glass ﬁber alloys via the same procedures described above. As shown in Table 3, the PEg-GMA is an excellent compatibilizer of PPS/nylon 6,6/ glass ﬁber alloys since the impact strength of alloy p is higher than alloy o due to the generation of strong van der Waal forces in between the epoxy group of PE-gGMA and the amine group of nylon 6,6 as well as the sulﬁde group of PPS. Moreover, chemical reaction between the nylon 6,6 and the PE-g-GMA may proceed from the amine addition , further promoting the compatibility of PPS/PA6,6 alloys. As shown in Tables 2 and 3, in addition, the impact strength of PPS/nylon 6,6/glass ﬁber alloys with PE-g-GMA (alloy p) is much higher than that of PPS/PET alloys with PE-g-GMA (alloy n), revealing that addition of Table 3 Summary of the experimental results of PPS/nylon 6,6/ glass ﬁber alloys Alloy Composition of PPS/nylon 6,6/glass ﬁber/PE-g-GMA (wt./wt./wt./wt.) Unnotched impact strength (kg/cm)a o p 100/50/45/0 100/50/45/12.5 78 >100 a Measured at 25 °C after aging at 240 °C for 231 h (the standard deviations = ±2%). nylon 6,6 and glass ﬁber can drastically increase the mechanical properties of PPS. 4. Conclusions In conclusion, grafting extrusion of epoxy-modiﬁed polyethylene (PE-g-GMA) was successfully performed and the percentage of grafting could be rapidly estimated by the linear calibration curve. With PE-g-GMA as a compatibilizer, PPS/PET and PPS/nylon 6,6/glass ﬁber alloys are homogenously dispersed and their unnotched impact strengths were effectively enhanced due to strong van der Waal forces between the epoxy group of PE-g-GMA and functional groups of polymers (i.e. the carboxyl as well C.-M. Chen et al. / Reactive & Functional Polymers 68 (2008) 1307–1313 as oxygen groups of PET, the sulﬁde group of PPS, and the amine group of nylon 6,6). Acknowledgements The authors acknowledge part of the ﬁnancial support of this work by National Science Council of the Republic of China under Contract NSC94-2216-E-009-026. References  D. Braun, U. Eisenlohr, Angew. Markromol. Chem. 55 (1976) 43.  R.A. Steinkamp, T.J. Grail, U.S. Patent 3,953,655, 1976.  N.G. Gaylord, M. Mehta, J. Polym. Sci., A 26 (1988) 1189. 1313  M. Tomescu, M. Dimonie, E. Calota, C. Ionescu, Mater. Plast. 15 (1978) 10.  B.E. Spivey, U.S.Patent 3,383,372, 1968.  T.C. Chung, Prog. Polym. Sci. 27 (2002) 39.  M.F. Diaz, S.E. Barbosa, N.J. Capiati, Polymer 43 (2002) 4851.  D.S. Rosa, C.G.F. Guedes, M.A.G. Bardi, Polym. Test. 26 (2007) 209.  R.R. Gallucci, R.C. Going, J. Appl. Polym. Sci. 27 (1982) 425.  K. Nakanishi, Infrared Absorption Spectroscopy, Holden-Day, San Francisco, 1962.  J.G. Martinez, R. Benavides, C. Guerrero, B.E. Reyes, Polym. Degrad. Stab. 86 (2004) 129.  T. Hisamatsu, S. Nakano, T. Adachi, M. Ishikawa, K. Iwakura, Polymer 41 (2000) 4803.  F.P. Tseng, J.J. Lin, C.R. Tseng, F.C. Chang, Polymer 42 (2001) 713.  N.C. Liu, H.Q. Xie, W.E. Baker, Polymer 34 (1993) 4680.  A.V. Pocins, Adhesion and Adhesive Technology: An Introduction, Hanser/Gardner Publications, New York, 1997.